Contents Preface xi Acknowledgments xiii CHAPTER 1 Silicon Carbide Overview 1 1.1 General Properties 1 1.1.1 Mechanical and Chemical Properties 2 1.1.2 Bandgap 2 1.1.3 Critical Field 2 1.1.4 Saturated Drift Velocity 3 1.1.5 Thermal Conductivity 3 1.1.6 Figures of Merit 4 1.2 History 4 1.2.1 Berzelius and Acheson 4 1.2.2 The Discovery of Polytypism 6 1.2.3 The First LED and the Lely Process 6 1.2.4 The Lost Decades 7 1.2.5 The Second Wave 7 1.2.6 The Third Wave 7 1.3 Crystalline Structure 8 1.3.1 Basic Structure 8 1.3.2 Polytypism 8 1.3.3 Impurities in Different Polytypes 9 1.4 Crystal Growth 11 1.4.1 Seeded Sublimation Growth 11 1.4.2 High Temperature Chemical Vapor Deposition 14 1.5 Epitaxial Growth 18 1.5.1 Chemical Vapor Deposition 18 1.6 Defects 21 1.6.1 Micropipes 21 1.6.2 Stacking Faults 22 1.7 Commercial Outlook 22 1.7.1 High-Frequency Applications 23 1.8 Summary 25 References 26 vii
viii Contents CHAPTER 2 High-Temperature SiC-FET Chemical Gas Sensors 29 2.1 Introduction 29 2.2 Detection Mechanism of Field-Effect Gas Sensors 30 2.2.1 Gas Sensing Principle 30 2.2.2 Detection of Different Molecules 31 2.2.3 Influence of Oxygen 34 2.2.4 Influence of Different Metals 35 2.2.5 Influence of Temperature 36 2.2.6 Sensor Arrays 36 2.3 Field-Effect Chemical Gas Sensor Devices 38 2.3.1 Capacitors 38 2.3.2 Schottky Diodes 38 2.3.3 The P-N Junction Diode 43 2.3.4 Field-Effect Transistors 44 2.4 Sensor Properties at Elevated Temperatures, Influence of Hydrogen 49 2.4.1 Influence of Hydrogen on Capacitors 50 2.4.2 Influence of Hydrogen on Schottky Diodes 51 2.5 More Sensor Properties 53 2.5.1 Speed of Response 53 2.5.2 Long-Term Stability 56 2.6 Experimental 57 2.6.1 Sample Preparation 57 2.6.2 Gate Metal Deposition 57 2.6.3 Mounting 58 2.6.4 Device Operation 58 2.7 Applications 59 2.7.1 Petrol Engine Exhausts 59 2.7.2 Diesel Engine Exhausts 60 2.7.3 Flue Gas Monitoring 61 2.8 Outlook and Conclusions 62 Acknowledgments 63 References 63 CHAPTER 3 Silicon Carbide Technology and Power Electronics Applications 69 3.1 DC-DC Conversion 69 3.1.1 SMPC Circuit Topologies and Operation 70 3.1.2 Silicon Carbide Devices in SMPC Applications 73 3.1.3 Other SiC Switches 78 3.1.4 SiC AC-DC Inverter Example 79 3.2 DC-AC Power Conversion 80 3.2.1 DC-AC Power Inverter 80 3.2.2 Inverter Control Techniques 81 3.2.3 SiC DC-AC Inverter Example 82 3.3 Pulsed-Power Applications 91 3.3.1 Thyristor Basics 92
Contents ix 3.3.2 Evaluation of SiC Thyristors for Pulsed-Power Switching 94 3.4 Thermal Management and High-Voltage Packaging 97 3.4.1 Hybrid Si-SiC Half-Bridge Module 98 3.4.2 Implementation Analysis of a High-Voltage SiC Bridge Rectifier Module 100 3.4.3 Electrostatic Analysis of a High-Voltage Package for SiC Devices 103 3.5 Summary 106 References 106 CHAPTER 4 Advances in Selective Doping of SiC Via Ion Implantation 109 4.1 Introduction 109 4.2 As-Implanted Profiles 114 4.2.1 Diagnostic Techniques 114 4.2.2 Random Implants 115 4.2.3 Channeled Implants 124 4.3 Implant Annealing 128 4.3.1 Annealing Concepts 128 4.3.2 Silane Overpressure Annealing Process 130 4.3.3 Implanted Ion Profiles After Annealing 136 4.3.4 Defect Evolution 140 4.3.5 Results of Electrical Activation 143 4.4 Technology Barriers and Suggestions for Future Work 147 References 148 CHAPTER 5 Power SiC MOSFETS 155 5.1 Introduction 155 5.2 SiC UMOSFET 156 5.3 SiC DIMOSFET 163 5.4 SiC LDMOS 169 5.5 Summary and Future Development 171 References 172 CHAPTER 6 Power and RF BJTs in 4H-SiC: Device Design and Technology 177 6.1 Introduction 177 6.2 Device Structures and Operation of Power BJTs 177 6.3 Design of the Epitaxial Power BJT 181 6.3.1 Design of the Collector Layer 181 6.3.2 Design of the Base Layer 183 6.3.3 Design of the Unit Cell 184 6.4 Process Integration 186 6.4.1 Process Sequence 186 6.5 1.2-kV Power BJTs 188 6.6 Design and Fabrication of UHF Transistors 192
x Contents 6.7 Future Work 199 References 200 About the Editors 203 Index 205
Preface Recently there have been numerous books written on SiC, which is a testament to the importance of this technology and its potential impact on society. A majority of these books attempt to comprehensively cover a specific aspect of the technology and do this by a set of in-depth chapters on a particular research topic, concept, or result. While this is an excellent means to convey important aspects of the technol- ogy, the intent of Advances in Silicon Carbide Processing and Applications is to be less expansive and focus in on two of the most promising applications of SiC tech- nology: gas and chemical sensing and electric vehicle motor drive and control. Hav- ing made this decision, we realized that the underlying device and processing issues that enable these application areas to be served by SiC technology should also be addressed. Hence a major portion of the book involves aspects of SiC technology in this key area, again with the intent (and hope) that the reader will be able to gain a broad and deep insight into the pacing issues of the technology as of this date. While there is no way to predict the wisdom of this strategy a priori, we have nonetheless tried to put ourselves into the shoes of potential readers of this book and carefully selected chapter topics that would best support this strategy. We hope that all who read this book will benefit from the somewhat different approach we have taken. We begin with an overview of SiC as of 2003, with an attempt to provide some predictions as to the market for the technology. We then immediately jump into the application chapters, first on gas sensors, which is clearly an area where SiC can gain a significant market share compared with traditional Si technology, followed by advances in electric motor drive where, again, SiC clearly has an advantage over Si due to its robust material properties. We then step back and discuss the all-important area of SiC ion implantation technology—this is key since the properties of the SiC lattice precludes the use of thermal diffusion to achieve planar selective doping over the surface of single-crystal wafers. After dis- cussing this topic, we then finish up with a discussion of recent advances in both SiC MOS and bipolar technology, both of which directly impact the sensor and motor drive applications. Attention was made to provide a large number references in the recognition that no single book can be fully exhaustive of such a broad subject such as SiC. xi
Acknowledgments It is with the most sincere gratitude that the editors of this book thank all of the chapter authors for their dedication and hard work in bringing this idea to fruition. Just as a work of art can be immediately appreciated by the viewer, without any understanding of the efforts expended to bring it about, so too is a well-written book easy to appreciate by the reader without an appreciation of the long hours of hard work that is involved. Special thanks go to our colleagues who reviewed spe- cific chapters of the book; their contribution has certainly improved the quality of each chapter. In particular, we thank John Wolan of the University of South Florida for his review of Chapter 2, Omar Manasreh for his review of Chapter 3, Nelson Saks of the Naval Research Laboratory for his review of Chapter 4, and Paul Chow of RPI for his review of Chapter 6. We wish to thank all of the SiC pioneers who have come before us and all of the present researchers in the field who have pushed the technology to the point where such a book project was warranted. Stephen E. Saddow would like to personally thank all of his current and former students, espe- cially in the SiC Group at the University of South Florida, for all of their dedication and hard work that made this book possible. Stephen E. Saddow Tampa, Florida Anant Agarwal Durham, North Carolina June 2004 xiii
CHAPTER 1Silicon Carbide Overview Olle Kordina and Stephen E. Saddow1.1 General Properties Silicon carbide (SiC) is a semiconductor material with highly suitable properties for high-power, high-frequency, and high-temperature applications. This almost worn-out opening statement may be found in many papers dealing with SiC. Yet, it cannot be left out because it really brings forward the essence of the material’s potential. Silicon carbide is a wide bandgap semiconductor material with high breakdown electric field strength, high saturated drift velocity of electrons, and a high thermal conductivity. In combination with these properties, a native substrate of reasonable size exists, and one may readily grow the material and dope it both n- and p-types. In addition, SiC, like silicon (Si), has SiO2 as its stable, native oxide. This fact is often overlooked but is key to any semiconductor technology, both from a processing perspective as well as opening up metal-oxide-semiconductor (MOS) device opportunities for SiC. Therefore, these properties make SiC ideally suited for a vast number of applications. In this chapter, we will discuss more details of these exciting properties and provide a realistic assessment of the material’s challenges that are actively being studied to date. Indeed, one has to recognize that the unique properties of SiC—its robust structure, wide bandgap, high-temperature stability and so forth—also make it a challenge to manufacture and process into working devices. Although these challenges are not insurmountable, one needs to be aware of their implications before deciding to choose SiC as the technology for a particular application. Therefore, the purpose of this book is to provide the reader with a realistic assessment of SiC as a technology one might select for a given application of inter- est. In this chapter, we will review material issues related to bulk and thin-film growth of SiC and then discuss some interesting applications of SiC. This will be fol- lowed by a discussion of one of the key process technologies that is absolutely essen- tial to SiC—selective doping via ion implantation. We will then provide an update of several key device technologies ranging from power electronic switch develop- ment to MOS transistors and finally high-power radio frequency (RF) and bipolar devices. The industrial application of SiC began with the blue light emitting diode (LED), which was very weak due to the indirect bandgap of SiC but was the only commercial blue electroluminescent light source at the time (the late 1980s). The SiC blue LED was soon surpassed in intensity by the gallium nitride (GaN)-based 1
2 Silicon Carbide Overview LED due to the direct bandgap of the III-nitrides. However, due to the lack of a native substrate for GaN, sapphire or SiC substrates were and are still used. The big- gest use of semiconductor-grade SiC is still for LEDs, but now it serves the role as the substrate for the active GaN layer rather than both the substrate and the active layer. Today there are high-frequency metal-semiconductor-field effect transistors (MES- FETs) offered commercially, as well as an emerging market for Schottky diodes made from SiC. We are still at the beginning of the SiC revolution, however, and the material’s full potential has yet to be realized. 1.1.1 Mechanical and Chemical Properties Silicon carbide is a very hard substance with a Young’s modulus of 424 GPa . It is chemically inert and reacts poorly (if at all) with any known material at room tem- perature. The only known efficient etch at moderate temperatures is molten KOH at 400–600°C. It is practically impossible to diffuse anything into SiC. Dopants need to be implanted or grown into the material. Furthermore, it lacks a liquid phase and instead sublimes at temperatures above 1,800°C. The vapor constituents during sublimation are mainly Si, Si2C, and SiC2 in specific ratios, depending on the temperature. 1.1.2 Bandgap The bandgap varies depending on the polytype between 2.39 eV for 3C-SiC to 3.33 eV for 2H-SiC . The most commonly used polytype is 4H-SiC, which has a band- gap of 3.265 eV . The wide bandgap makes it possible to use SiC for very high- temperature operation. Thermal ionization of electrons from the valence band to the conduction band, which is the primary limitation of Si-based devices during high- temperature operation, is not a problem for SiC-based devices because of this wide bandgap. 1.1.3 Critical Field For power-device applications, perhaps the most notable and most frequently quoted property is the breakdown electric field strength, Emax. This property deter- mines how high the largest field in the material may be before material breakdown occurs. This type of breakdown is obviously referred to as catastrophic breakdown. Curiously, the absolute value of Emax for SiC is frequently quoted as the relative strength of the Emax against that of Si. Most discussions on this subject note that Emax of SiC is 10 times that of Si. As with Si, there exists a dependence of Emax with doping 16 −3 concentration. Thus, for a doping of approximately 10 cm , Emax is 2.49 MV/cm, according to a study by Kostantinov et al. . For Si, the value of Emax is about 0.401 MV/cm for the same doping . As can be seen, the value for SiC is only about a fac- tor of six higher than that of Si and not the often-claimed 10 times higher critical field strength. Why the discrepancy? It is more correct to compare the critical strengths between devices made for the same blocking voltage. Thus, an Si device constructed for a blocking voltage of 1 kV would have a critical field strength of
1.1 General Properties 3 about 0.2 MV/cm, which should be compared with the 2.49 MV/cm of SiC. This is where the order of magnitude larger breakdown field spec comes from. 1.1.4 Saturated Drift Velocity For high-frequency devices, the breakdown electric field strength is not as important as the saturated drift velocity. In SiC, this is 2 × 10 cm/sec [5, 6], which is twice that 7 of Si. A high-saturated drift velocity is advantageous in order to obtain as high- channel currents as possible for microwave devices, and clearly SiC is an ideal mate- rial for high-gain solid-state devices. 1.1.5 Thermal Conductivity The second most important parameter for power and high-frequency device appli- cations is the material’s thermal conductivity. An increase in temperature generally leads to a change in the physical properties of the device, which normally affects the device in a negative way. Most important is the carrier mobility, which decreases with increasing temperature. Heat generated through various resistive losses during operation must thus be conducted away from the device and into the package. It is often quoted that the thermal conductivity of SiC is higher than that of cop- per at room temperature. There are even claims that it is better than any metal at room temperature . The thermal conductivity of copper is 4.0 W/(cm-K) . That of silver is 4.18 W/(cm-K) . Values of the thermal conductivity as high as 5 W/(cm-K) have been measured by Slack  on highly perfect Lely platelets. More detailed studies have been made where the thermal conductivity in the dif- ferent crystal directions have been determined for SiC (see Table 1.1 ). As can be seen, there is a dependence on the purity of the crystal as well as on the crystal direc- tion. At the time of this study, the material was not of the high quality we see today, and more sophisticated techniques have been developed to measure thermal con- ductivity. Thus, as higher-quality material has been grown, values close to the theo- retical values have been measured using the laser flash technique . High-purity semi-insulating (SI) SiC material has the highest reported thermal conductivity with a value of 4.9 W/(cm-K). Lower values are measured for the doped crystals but they are all above 4 W/(cm-K) at room temperature . Table 1.1 The Thermal Conductivity of SiC Carrier Sample Concentration Thermal Conductivity Type Direction (cm−3) (W/cm K) 298K 373K 4H SI // c SI 3.3 2.6 4H n // c 2.0 E18 3.3 2.5 4H n ⊥c 5 E15 4.8 2.9 6H n // c 1.5 E18 3.0 2.3 6H n // c 3.5 E17 3.2 2.3 6H n ⊥c 3.5 E17 3.8 2.8 6H p ⊥c 1.4 E16 4.0 3.2 Slack ⊥c ~ 1 E17 ~5 ~3 Source: .
4 Silicon Carbide Overview 1.1.6 Figures of Merit There have been several attempts to summarize the importance of various material properties to enable comparisons between materials for high-frequency and high- power applications. Johnson suggested a figure of merit, the so-called Johnson Fig- ure of Merit (JFOM), which considers the potential power handling and high- frequency capability of a device. The JFOM takes into account the critical field and saturated drift velocity, as shown in the following equation . EB v 2 2 JFOM = sat (1.1) 4π 2 where EB and vsat are the breakdown field and saturated drift velocity, respectively. Unsatisfied with the JFOM ability to take the material’s thermal properties into account, which, as mentioned, are specifically apparent during high-frequency operation, Keyes proposed another figure of merit, the Keyes Figure of Merit (KFOM) : cv sat KFOM = κ (1.2) 4πε where κ, c, and ε are the thermal conductivity, the speed of light in vacuum, and the dielectric constant, respectively. Unfortunately, neither of these equations is particularly accurate for power devices and consequently Baliga proposed a figure of merit for low-frequency appli- cations, called the Baliga Figure of Merit (BFOM) : BFOM = εµE B 3 (1.3) where µ is the carrier low-field mobility. In Table 1.2, the figures of merit for the two most common SiC polytypes are compared with Si and GaAs. All values are normal- ized to Si.1.2 History 1.2.1 Berzelius and Acheson Jöns Jacob Berzelius is mostly known for his discovery of Si; however, he was the first person who more than likely synthesized SiC. In 1824 he published a paper where he speculated that there was a chemical bond between Si and carbide (C) in Table 1.2 Figures of Merit for Si, GaAs, and the Two Most Common SiC Polytypes (Values Are Normalized to Si) Material JFOM KFOM BFOM Si 1 1 1 GaAs 9 0.41 22 6H-SiC 900 5.0 920 4H-SiC 1,640 5.9 1,840
1.2 History 7 1.2.4 The Lost Decades In 1958, the first SiC conference was held in Boston, Massachusetts. However, after this, the interest in SiC rapidly declined and the 1960s and 1970s are characterized by a low interest in SiC. Research was still ongoing, mainly in the former Soviet Union. In the United States, the work done by Westinghouse and the University of Pittsburgh is primarily notable. Indeed, the photoluminescence studies made by Choyke, Patrick, and Hamilton are still very relevant and often cited . 1.2.5 The Second Wave In the late 1970s, a very important invention—the seeded sublimation growth [22, 23]—was made in Russia by Tairov and Tsvetkov. Unlike the Lely process and the growth in the Acheson voids, where the growth is conducted under close-to-uniform thermal conditions, Tairov and Tsvetkov introduced a seed crystal and forced mate- rial transport from the source to the seed by a thermal gradient (Figure 1.3). The growth rates increased markedly and seeds of larger diameters and lengths could be made. The produced boules could be sliced and polished. The SiC wafer was born. Another major invention that came only two years later was the ability to grow epitaxial SiC on Si substrates . Research on SiC gained new speed, but it was a spark that never really caught on. However, there was generally a greater awareness of SiC and its potential, which was important for the years to come. 1.2.6 The Third Wave In 1987, another milestone occurred when high-quality epitaxy could be made at low temperatures on off-axis substrates using “step-controlled epitaxy” . Cree, Inc., was founded in 1989 as a result of this breakthrough. It manufactured the first commercial blue SiC LEDs and began to sell SiC wafers as well. At the same time, the company generated demonstrators for power devices and high-frequency devices. This was the beginning of the third and last wave of SiC. Along with improved epitaxy, continuous improvement of the diameter and quality of the wafers, and device milestones, this third wave has not died out but continues to grow in strength. The commercial potential of SiC has to date mainly been in the materials arena. SiC is used as substrate for LEDs made from GaN, which is the largest market of semiconductor-grade SiC. Recently Infineon launched its Schottky diode product T2 < T1 T1 > 2,000ºC Figure 1.3 The seeded sublimation growth or modified Lely growth invented by Tairov and Tsvetkov.
8 Silicon Carbide Overview line made from SiC and Cree has also come out with a Schottky diode as well as high-frequency MESFETs. The future for SiC looks very bright indeed now that commercial products have hit the marketplace!1.3 Crystalline Structure 1.3.1 Basic Structure The basic building block of a silicon carbide crystal is the tetrahedron of four carbon atoms with a silicon atom in the center (Figure 1.4). There also exists a second type rotated 180° with respect to the first. The distance between the carbon and silicon atom is 1.89Å and the distance between the carbon atoms is 3.08Å . SiC crystals are constructed with these units joining at the corners. 1.3.2 Polytypism Silicon carbide exhibits a two-dimensional polymorphism called polytypism. All polytypes have a hexagonal frame of SiC bilayers. The hexagonal frame should be viewed as sheets of spheres of the same radius and the radii touching, as illustrated in Figure 1.5. The sheets are the same for all lattice planes. However, the relative posi- tion of the plane directly above or below are shifted somewhat to fit in the “valleys” of the adjacent sheet in a close-packed arrangement. Hence, there are two inequiva- lent positions for the adjacent sheets. By referencing the possible positions as A, B, and C, we can begin constructing polytypes by arranging the sheets in a specific repetitive order. Thus, the only cubic polytype in SiC is 3C-SiC, which has the stacking sequence ABCABC… The simplest hexagonal structure we can build is 2H, which has a stacking sequence ABAB… The two important polytypes, 6H-SiC and 4H-SiC, have stacking sequences ABCACBABCACB… and ABCBABCB…, respectively. The number in the notation of the resulting crystal structure determines the number of layers before the sequence repeats itself, and the letter determines the result- ing structure of the crystal: C for cubic, H for hexagonal, and R for rhomohedral. C C 1.89Å Si Si 3.0 8Å Figure 1.4 The characteristic tetrahedron building block of all SiC crystals. Four carbon atoms are covalently bonded with a silicon atom in the center. Two types exist. One is rotated 180° around the c-axis with respect to the other, as shown.
1.3 Crystalline Structure 9 A A B B A A A C C B B B A A A A C B B A A A Figure 1.5 Illustration of three close-packed planes of spheres. The first layer is a layer of “A” atoms, followed by a layer of atoms on a “B” position, with a layer of atoms on “C” positions on top of that. The resulting structure in this example is 3C-SiC. All polytypes are SiC of equal proportions of silicon and carbon atoms, but due to the fact that the stacking sequence between the planes differs, the electronic and optical properties differ. The bandgap is, for instance, 2.39 eV for 3C-SiC, 3.023 eV for 6H-SiC, and 3.265 eV for 4H-SiC . The unit cell for the different polytypes will naturally vary, as will the number of atoms per unit cell. This will affect the number of electronic bands and the phonon branches for a given polytype. 1.3.3 Impurities in Different Polytypes A very striking and beautiful feature of polytypism is the behavior of impurity atoms. In Figure 1.6, it may be seen that the sites are not equivalent in the hex- agonal polytypes 6H-SiC and 4H-SiC. The difference is in the second-nearest neighbors. A nitrogen atom substituting a carbon atom in the lattice can either occupy a “k” site or an “h” site in 4H-SiC. The k site is a lattice site that displays cubic sym- metry, whereas the h site has hexagonal symmetry. The immediate vicinity of a nitrogen atom on either site is the same, but the second-nearest neighbors to the sites are different, which creates a slightly different core binding energy. Thus, 4H-SiC has two binding energies for the nitrogen donor, which has consequences when designing devices. 6H-SiC has three energy levels for nitrogen and 3C-SiC has only one. More complex polytypes such as rhombohedral (15R-SiC) has no less than five binding energies, although only four have been identified. The photoluminescence (PL) spectrum in Figure 1.7 shows a number of lines related to nitrogen-bound excitons and free excitons. SiC has an indirect bandgap, thus the exciton-related luminescence is often assisted by a phonon. Bound exciton luminescence without phonon assistance can, however, occur because conserva- tion in momentum can be accomplished with the help of the core or the nucleus of the nitrogen atom. That is why the zero phonon lines of the nitrogen atom are seen, denoted P0 and Q0, in the spectrum but not the zero phonon line of the free exciton.
10 Silicon Carbide Overview   B  A C B A A h C C C h k2 k B B B k k1 k A A A Figure 1.6 The three most common polytypes in SiC viewed in the  plane. From left to right, 4H-SiC, 6H-SiC, and 3C-SiC; k and h denote crystal symmetry points that are cubic and hexagonal, respectively. The binding energies for the hexagonal and cubic nitrogen impurities are 59 meV and 102 meV, respectively . According to the effective mass approximation , the binding energy of an electron bound to a nitrogen atom in 4H-SiC would be: Z 2 m* E D = 136 . eV ≈ 607 meV . (1.4) n 2 ε 2 m0 r 1 P76 P96 I76 + P68 P95 + I104 I107 0.75 Normalized PL Intensity P107 Q0 0.5 I96 Q76 I95 P104 I46 P46 0.25 P33.2 I41 P51 P0 I51 I68 I33.5 0 3,780 3,830 3,880 3,930 3,980 Wavelength (Å) Figure 1.7 Near-band-edge photoluminescence spectrum of 4H-SiC showing the bound exciton- related luminescence denoted Ph and Qh (where h is the energy in meV of the phonon involved in the transition) and free exciton-related luminescence denoted Ih. (Data provided by Docent Anne Henry at Linköping University.)
1.4 Crystal Growth 11 where m* and εr are the effective mass and dielectric constant, respectively. Z is the charge that is equal to 1 in this example and n is an integer equal to 1 for the ground state. The discrepancy between the actual binding energy, 59 meV, and what the effective mass approximation predicts is taken up by the core and is referred to as the central cell correction. In this example, the central cell correction is about 53 meV. Defects with large central cell correction have very localized wave functions. The larger the correction, the more localized the wave function and the higher the probability of interaction between the core (or central cell) and the electron and/or the exciton bound to the defect. Hence the reason why the P0 line is so much smaller than the Q0 line in the spectrum, as well as the reason why the phonon replicas to the Q-line, is simply a matter of probability, since the central cell correction is so much larger for a nitrogen defect on a cubic site than a hexagonal site. A useful feature of photoluminescence that is not limited to but very apparent in SiC is the ratio between the free exciton and bound exciton luminescence, which can give an accurate determination of the level of doping once properly calibrated . In a perfectly pure crystal, the electron-hole pairs created through the absorption of above bandgap photons would bind together to form free excitons. These would move freely in the crystal until they recombine and possibly generate some light in the recombination process. If we do the same in a crystal with a small amount of nitrogen in it, some of the free excitons will likely hit on a nitrogen defect, which will attract the free exciton. The free exciton will lose some of its energy and bind to the defect center into a four-particle complex called the bound exciton. The four particles are the electron-hole pair of the free exciton, the electron of the nitrogen defect, and the core of the nitrogen atom. The bound exciton will, of course, also recombine and emit some light. Thus, by comparing the ratio between the free exci- ton and bound exciton luminescence, the doping level can be determined. The paper by Henry et al.  continues to describe how PL may be used at higher doping levels where the free exciton is no longer seen by comparing the Q0 line and the P76 line. In the very high doping range, the authors correlated success- fully the position of a broad nitrogen-related luminescence band with the doping concentration.1.4 Crystal Growth 1.4.1 Seeded Sublimation Growth 188.8.131.52 General Principle As previously mentioned in Section 1.2, Tairov and Tsvetkov  invented seeded sublimation growth in 1978. The technique is almost exclusively used today to manufacture SiC wafers. The principle is simple. A graphite crucible is partially filled with SiC powder and a seed is attached on the lid of the crucible. The whole system is closed and heated up to temperatures above which SiC starts to sublime appreciably. A thermal gradient is applied such that the seed is slightly colder than the powder source. Material will thus transport from the source to the seed where it will condense. The principal constituents during sublimation are Si, Si2C, and SiC2 and the ratio between them is determined by the temperature.
1.4 Crystal Growth 13 It is hard to understand the tremendous interest in the vanadium doped crystals since, in 1993, the Westinghouse Science and Technology Center was already pro- ducing 6H-SiC wafers with resistivities as high as 10 Ω-cm without the introduc- 5 tion of impurities by simply growing the crystals as purely as it could achieve . It is particularly surprising in view of the fact that it was the same group that first introduced the vanadium doping. It is unfortunate that they did not realize that the most promising and much superior approach was to continue to improve the purity of the crystals as much as possible. Other than poor crystalline quality and yield problems, there was one more problem with the vanadium doped SI SiC wafers; they did not work for high- frequency applications due to excessive trapping of electrons. A very elegant dem- onstration of this trapping can be seen in the publication by Sghaier et al., where the degradation in performance of the high-frequency device was clearly seen and it concluded that the cause for the trapping was the vanadium doped substrate . Then, in 1999, the high-frequency community, in desperate need of better semi-insulating substrates, regained their confidence due to some interesting results where very pure, vanadium-free crystals had been grown that displayed SI behavior . The authors found a deep level with an activation energy of 1.1 eV, though they had no clear identification of the identity of the defect. However, they specu- lated that it was intrinsic in nature. The resistivity was outstanding, demonstrating a resistivity in excess of 107 Ω-cm at 300°C, which is high enough for most power RF applications. Another even more interesting development was occurring at the same time. This was the development of a new growth technique, called the High Temperature Chemical Vapor Deposition (HTCVD) technique , that produced crystals that were intrinsically semi-insulating. In a paper by Ellison et al. , the authors reported on a defect with an activation energy of 1.15 eV yielding an extrapolated room temperature resistivity in excess of 109 Ω-cm. Further work showed that several intrinsic defects can contribute to the semi- insulating properties of the crystal, such as Si-vacancies, C-vacancies, and C-antisites. Typically, the resistivity of semi-insulating crystals containing predomi- nately Si-vacancies is lower and the activation energy of the responsible defect is less than 1.1 eV, whereas crystals with predominately C-vacancies content have higher resistivities and the activation energy is around 1.4 eV . Lately, photo-electron paramagnetic resonance (EPR) measurements revealed that the carbon vacancy acts as a deep donor with an activation energy of 1.47 eV . This provides to date the strongest evidence that C-vacancies play a role in SiC similar to the well-known EL2 deep level in GaAs for producing high-purity semi-insulating wafers. Now, 2-inch SI wafers without vanadium doping are sold commercially from several sources. Vanadium doped crystals will rapidly disappear and soon only be used as displays in museums or as book rests. 184.108.40.206 Prospect A lot of research is being conducted on the seeded sublimation growth technique. The material properties are improving steadily and there should be no reason for worries. Yet, one worry is the need for off-axis substrates for high-quality epitaxial
14 Silicon Carbide Overview growth. The current standard of 8° off-axis from the  plane on the 4H-SiC wafers was introduced in 1995 by Cree, since it had seen an improvement in the epi- taxy when the off-axis angle was increased from 3.5° (which is still the standard mis- cut for 6H-SiC). At that time, only 30-mm wafers were available commercially, and it was not a big problem to slice the wafers somewhat more off-axis. It was only a matter of 4-mm lost material in total from the grown boule. On a 100-mm wafer, the amount of lost material is no less than 14 mm. Considering that most boules in the world are grown on-axis parallel to the c-axis and that the length is limited to approximately 25–30 mm, it is going to cause significant heartache to slice the boule 8° off-axis and lose half of the material. The trend must be to reduce the off-axis angle. Fortunately, if we peek at what has happened previously in the Si and GaAs worlds, the standard was to use off-axis substrates initially, but as the material quality improved, the need for off-axis sub- strates was reduced and on-axis substrates are now used for epitaxy. This is likely going to be the trend in SiC too. The need for better epitaxial procedures and higher-quality substrates than what is available today is important. Boule lengths are also likely to increase. More powder may be introduced into the growth chamber, however, thermal considerations become an issue as the boules increase too much in length. Even if the surface is kept at constant distance in the chamber, the distance from the source will vary as the material is depleted and the growth conditions change. The source material will release excess silicon in the beginning of the growth cycle and be more carbon-rich in the end due to preferential depletion of silicon. This is a known problem and it is a matter of detailed control and an understanding of the dynamic transport mechanisms in combination with thermodynamics. Never- theless, the result is invariably that SiC boules grown by seeded sublimation growth are Si-rich in the beginning and C-rich near the end, which creates yield issues. Simu- lation of the process is necessary to improve the situation. The turnaround time for a boule growth run is several days. It takes time to pre- pare the source, load the crucible, attach the seed, evacuate the system carefully, gradually heat up the crucible under controlled conditions, and finally grow the boule and then cool down. The turnaround time itself is not a problem, however, the cost of manufacturing a wafer needs to decrease so the price of the wafers can be reduced in order for SiC to gain acceptance in the market. Seeded sublimation growth is a mature and needed tool for the SiC industry today. There are still major challenges. Specifically, boules will need to be grown on off-axis substrates, or the off-axis angle needs to be eliminated, which will only be possible if a combined effort of improving wafer quality, polishing procedures, and epitaxial procedures is pursued. 1.4.2 High Temperature Chemical Vapor Deposition In 1995, a new technique, called HTCVD, was presented for the growth of SiC boules. This technique uses gases instead of a powder as source material. It was first presented at ICSCRM ’95 in Kyoto, Japan, but the first publication of HTCVD in a journal was in 1996 . More recent publications are available where the tech- nique is better described .
1.4 Crystal Growth 15 220.127.116.11 General Principle The HTCVD apparatus can be described as consisting of three separate zones: An entrance zone, a sublimation zone, and a growth (or condensation) zone. The gases used are mainly silane, ethylene, and a helium carrier. The carrier flow is very low. A schematic of the HTCVD system is shown in Figure 1.9. Silane and ethylene are present at very high concentrations so that homogene- ous nucleation dominates the process. As the gases enter into the hot part of the injector, the silane will decompose and form small Si liquid droplets or solid micro- crystals, depending on the temperature. The ethylene will also take part in the reac- tion, forming microparticles of SixCy. It has been noted  that even a small addition of hydrocarbons converts the Si droplets to stable particles of SixCy (or non- stoichiometric SiC). The stability may, in a hand-waving circumstantial way, be intuitively understood from a solubility point of view. The solubility of carbon in silicon is very low, thus, when carbon is added to the Si droplets, the phase will be solid rather than liquid. The process can work without additions of a hydrocarbon, in which case the carbon is supplied through a reaction between the hot silicon and the graphite walls. This is usually not the preferred growth mode and additions of hydrocarbons are needed to obtain a high growth rate. The formed microparticles of SixCy will move into the hot chamber or the subli- mation zone with the aid of the inert helium carrier gas. Once in the sublimation zone, the microparticles will sublime to form Si, Si2C, and SiC2, as in the case of seeded sublimation growth. A thermal gradient is applied, as illustrated in Figure 1.9, so that the sublimed species will condense on the seed, as in the case of seeded sublimation growth. There are similarities between seeded sublimation growth and HTCVD in that solid particles sublimate in the reactor and the vapor condenses on a seed crystal maintained at a lower temperature. However, the differences are quite dramatic and the outcome even more so. Take, for instance, the dynamics governing the growth Growth zone Sublimation zone Entrance zone Axial temperature Figure 1.9 HTCVD process. Microparticles are formed in the inlet region of the system and trans- ported to the sublimation zone, where the particles sublime to finally condense on the growth sur- face.
16 Silicon Carbide Overview rate. The heating of the particles in the sublimation zone must be efficient so that they sublime properly. Insufficient sublimation results in particles appearing as “smoke” coming out from the crucible. This is obviously not a good scenario and material quality, as well as growth rate, will suffer. The growth rate is naturally influenced by the amount of input precursors, how- ever, too high concentrations will give rise to too large nuclei, which will be difficult to sublime. As may have been deduced, if the thermal gradient between the seed and the sublimation zone is increased, the potential for sublimation will increase so that larger microparticles may be sublimed, thus larger amounts of precursors may be introduced and the growth rate will increase. The process is usually carried out at somewhat reduced pressures, though not at as low a pressure as seeded sublimation growth, where the pressure is greatly reduced to aid the material transport. HTCVD has its own material transport through the small but steady flow of helium, so reduced pressure is not needed to enhance growth species transport. However, the lower pressure will result in smaller particle sizes due to a suppression of homogeneous nucleation. Lowering the pres- sure will thus increase the maximum amount of precursors without observing “smoke” at the outlet. Thus, there are several ways to improve the growth rate, as can be seen. But in the end it all comes down to the size of the particles that need to be sublimed in the subli- mation zone. Typical maximum growth rates are in the order of 0.8 mm/hr–1 mm/hr. What is also interesting about the HTCVD is the material transport. Why does the silane not decompose and grow directly on the walls of the inlet? There are two reasons for this. First, the injector is a coaxial injector, as illustrated in Figure 1.9 . The silane and ethylene are transported in the inner tube, whereas there is only carrier gas in the outer tube. Thus the silane will not be in close proximity with a wall when it decomposes and will preferentially form nuclei through homogeneous nucleation. Second, the ethylene will make these particles very stable and hence they will not be prone to growth on the walls at all. As is well known, when hydrocarbons transported in an inert gas such as helium are heated, carbon or pyrolytic graphite will deposit on the walls. In the HTCVD, the ethylene helps make the particles stable and, in doing so, carbon is transported into the chamber together with the silicon. It is a sort of symbiosis in the transport between the silicon and carbon. 18.104.22.168 Material Properties One of the prime advantages of the HTCVD approach is the resulting crystal prop- erties. Due to the high purity of the gases, the material comes out intrinsically semi- insulating. Also, since the source material is produced on demand, the stoichiometry can always be kept the same, unlike the case with seeded sublimation growth. This will improve the yield of the grown material. It is also interesting to note that the technique is shown to reduce micropipes by 80% during each run . The micropipes close at the interface by some type of hol- low core-closing effect. Very low micropipe densities have been recorded using this technique, which is clearly much faster in improving material quality than seeded sublimation growth.
1.4 Crystal Growth 17 The resistivity of the SI wafers has been measured to be in excess of 10 Ω-cm at 11 room temperature . As mentioned earlier, a deep level defect was found to have an activation energy of 1.4 eV. MESFETs manufactured on these wafers show an increased performance in the sense of reduced trapping, which the authors explain as being primarily due to a reduction of the shallow impurities in the material. 22.214.171.124 Challenges Some of HTCVD’s initial challenges have been solved. For example, using a coaxial injector solved the blocking of the inlet. Another issue is the purity of the graphite material, which may be overcome using properly coated graphite crucibles. The outlet is a major problem because the material grows not only on the sur- face of the crystal but also around it and on the walls. When the outlet blocks, the- growth must be interrupted and hence the length of the crystals is limited. Work is ongoing to solve this specific issue and it has, to some extent, been fruitful. Crystals with a length in excess of 15 mm have been grown [A. Ellison, private communication]. New problems will arise as the crystal increases. It will, for instance, be neces- sary to pull the crystal during growth so that the growth surface remains at the same position in the crucible. When the crystals become long the thermal profile may change and will need to be controlled. Fortunately these are all problems that can be easily managed with proper engineering design and process simulation. As a result, there appear to be no real limitations to this approach. The growth rates today can be approximated to about 1 mm/hr, which means that roughly 20 mm of material may be grown each day, including 4 hours for the turnaround heat-up and cool-down time. Although this is better than what the seeded sublimation growth can achieve, growth rates will need to be increased fur- ther to drive wafer costs down. The cost of manufacture is often used as an argument against HTCVD. The reactors are, as may be understood, significantly more complex and hence also more expensive, compared with seeded sublimation growth. Graphite materials are some- what more expensive for HTCVD, whereas the gases are likely to be less expensive than high-purity powder material in bulk quantities. However, with a potentially higher throughput when using the HTCVD technique, and provided the volumes are high, it will actually be less expensive to use this technique than seeded sublima- tion growth since the cost will largely be driven by volumes. The cost comparison becomes even more favorable for HTCVD if the improved yields of low micropipe material, particular low micropipe SI material, are taken into account. However, such comparison is a meaningless exercise. A comparison of silicon, sapphire, GaAs, or other established materials, rather than other SiC growth tech- niques, should occur instead. The blue and white LEDs can, for instance, be made on either sapphire or SiC substrates. From a performance point of view, there appear to be advantages with the SiC substrate but the substrate cost is lower on sapphire, therefore making it the most-used substrate. Granted, once larger substrates of SiC are made available, it is doubtful that the LED cost will be lower on sapphire. Ultimately, SiC will not only be going up against sapphire but also against such giants as silicon and GaAs, which will require significant cost-reduction measures
18 Silicon Carbide Overview in the materials growth for SiC to become a viable technology. HTCVD is clearly a step in the right direction, but the SiC community still has a long way to go in this regard.1.5 Epitaxial Growth Several techniques for epitaxial growth exist today and it is therefore beyond the scope of this chapter to explain all of them. Chemical vapor deposition (CVD) is the only technique that is used for commercial applications of SiC and the description of epitaxy will be limited to this technique. Several different types of CVD reactors exist. The cold wall design, which used to be the most common type of reactor, is now less frequently used and the hot-wall reactor has filled its place. Some new and interesting concepts exist as well. These are referred to as chimney-type reactors. The main difference between the hot- or old-wall type reactors and the chimney-style reactor is the transport of materials, which will be explained in the following sections. 1.5.1 Chemical Vapor Deposition CVD of SiC normally uses silane and a hydrocarbon as the precursor gases and a hydrogen carrier gas. The gases pass over a heated graphite susceptor that is coated by SiC or tantalum carbide (TaC). The velocity of the gases is high but it is always laminar flow. Over the susceptor there will be a boundary, or stagnant, layer where the velocity gradient decreases to zero. As the gases are heated, the silane and hydrocarbon will decompose and the species will diffuse through the boundary layer to grow on the reactor walls or on the substrate. A comprehensive study of this may be found in a paper by M. Leys and H. Veenvliet . The concentration of precursor gases will decrease with respect to the flow direction over the susceptor due to the consumption of growth species, which results in a tapered layer thickness. This effect is known as depletion. To compensate for the depletion it is common to taper the susceptor such that the velocity of the gases increases along the flow direction over the susceptor and thus the boundary layer will be pushed downward, resulting in a shorter diffusion for the active species to the substrate. It is sometimes not enough to taper the susceptor to achieve good homogeneity of thickness and doping, hence other more complicated measures are applied, such as rotation of the substrate as described in the literature . In this paper, the authors also use a blend of argon and hydrogen as carrier gas, which has been shown to be advantageous to achieve better homogeneity . The flow of hydrogen is generally very high and the pressure is reduced. This is not so much on account of the flow dynamics but more due to reducing the homoge- neous nucleation of Si, which is significant when silane is used. The silicon cluster formation was first noticed and studied in detail by Rupp et al. in a single wafer Emcore reactor with a very high thermal gradient .
1.5 Epitaxial Growth 19 126.96.36.199 Doping Control This can be done by introducing nitrogen for n-type and trimethylaluminum (TMA) for p-type layers. To obtain a better range of doping, it has been elegantly demon- strated that by changing the C/Si ratio of the input gases the doping concentration will change without changing the flow of nitrogen or TMA. This effect is known as site competition . Unfortunately, when changing the stoichiometry, the mor- phology is affected somewhat and it is therefore not always desirable to do this if thick layers are to be grown. When doping is used and multiple layers are grown with different carrier type and conductivity, it is important that the doping level decreases rapidly after the source of the dopant is shut off. Otherwise one does not achieve abrupt junctions. This is known as the memory effect and it can be reduced by various tricks. For instance, one can vary the stoichiometry, provide a short purge without any dopant but continue to flow the normal precursor gases, or even perform an in-situ etch back before the next layer is grown. Although an Al memory effect was a concern in the early 1990s, this problem has been solved and it is no longer a concern. 188.8.131.52 Hot-Wall Reactor Prior to the introduction of hot-wall reactors in 1993 , thick, low-doped layers for very high voltages had not been achieved. This type of reactor proved it possible to grow very thick, low-doped layers of good morphology and high quality, which are needed for high-voltage power devices . Hot-wall CVD reactors have become increasingly popular due to the ease of obtaining high- quality layers. The stochiometry is usually selected with respect to optimum morphology and doping is varied by changing the partial pressures of the dopants. The reactor also displays a remarkably high uniformity in both thickness and doping. Even without wafer rotation, uniformities as tight as 1% in thickness and 2% in doping have been reported . More recently, rotation has been introduced, primarily to increase the capacity (i.e., to have the same high uniformity over several wafers ). The reproducibility was also reported to be very good, within ±10% in doping. The behavior of the hot-wall reactor has been investigated thoroughly. A short but comprehensive study by Wagner and Irmscher captures the main points . 184.108.40.206 Multiwafer Reactors Wafer rotation, as previously mentioned, has been introduced in the hot-wall reac- tor (see Figure 1.10), which gives it a capacity of 3 × 2-inch (that is, three 2-inch wafers can be run simultaneously to increase reactor throughput). The uniformity in this reactor is routinely 1–2% in thickness and 5–7% in doping [Rune Berge, Epi- gress, private communication]. Aixtron has manufactured both a cold-wall planetary reactor and a hot-wall planetary reactor for 7 × 2-inch wafer capacity or 5 × 3-inch. The cold-wall reactor has provided very good uniformities and its performance has been described in
20 Silicon Carbide Overview Figure 1.10 The hot-wall reactor with a 3 × 2-inch rotating platter. The mode of rotation is gener- ally gas-foil rotation. several papers . For the 7 × 2-inch reactor, they report on thickness uniformities around 4% and doping uniformities of 5% and 7%, depending on the doping level. The 7 × 2-inch hot-wall version has shown outstanding uniformities and high material quality . Uniformities in thickness of 0.4%, and doping of 5–6% have been demonstrated. Wafer-to-wafer uniformities are 0.6% in thickness and 3.6% in doping, which are outstanding results. Results for the 5 × 3-inch version of the same reactor are meager but the hot-wall version of the 5 × 3-inch reactor behaves much the same as the 7 × 2-inch (i.e., approximately the same uniformities [Rune Berge, Epigress, private communication]. 220.127.116.11 The Chimney Reactor An elegant new reactor concept for the growth of SiC epitaxial layers was intro- duced by Ellison et al. [34, 53] and is called the chimney reactor. This technique is similar to the HTCVD technique in that it is a vertical system and the material trans- port is achieved by allowing large clusters of Si to form. This is achieved by reducing the carrier flow, which thereby increases the partial pressure of the precursors. Hydrogen is used as the carrier gas but, again, only very small flow rates are required. The silicon clusters are formed in the inlet region at relatively low temperatures. As the temperature increases the formed Si clusters will thermally decompose and be available for growth. This is very similar to HTCVD; however, in this case there is no sublimation, only a decomposition of the Si clusters. Very high growth rates and outstanding purity has been achieved using this technique. Growth rates between 15–50 µm/hr and background doping in the low 1013 cm−3 have been reported by Zhang et al. . Typically, the temperatures used for growth are somewhat higher than those used in regular CVD, however, it need not be much higher. The high growth rates are obtained at higher temperatures as the dissociation of the Si clusters is more efficient.
1.6 Defects 21 Other groups have also worked on the same concept. Specifically, Tsuchida et al. have achieved very good results using this technique . Their reactor is heated through radiation using a cylindrical heating element surrounding a wedge-shaped substrate holder. The substrate temperature is lower (around 1,600°C) than what is usually used for chimney reactors but the surrounding heating element is signifi- cantly hotter. Kimoto et al. has also achieved high-quality results using the chimney tech- nique. They report doping concentrations below 1013 cm−3 .1.6 Defects It is important to discuss the major defects present in SiC. The intent is not to create an encyclopedia of SiC defects but rather highlight two that have become the favor- ite lament of device researchers and which create significant heartache and debate. 1.6.1 Micropipes In previous sections, micropipes have been discussed, and these are indeed the most important defect present in SiC. Micropipes may be caused by several screw disloca- tions bunching together to form a giant screw dislocation, making it energetically favorable to open up a hollow core in the center . A different way of forming micropipes may be simply by system contamination, where particles are trapped in the growing crystal, thus forming a micropipe, as described by Augustine et al. . The third way micropipes form, according to the same authors, is by vacancy con- densation at a helical dislocation. Micropipes are basically a hollow core penetrating the entire wafer along the c-axis direction. Placing any device directly on top of the micropipe is bound to cause failure. These defects are particularly disturbing for large-area devices such as high-power devices because the probability of placing your device on a micropipe increases, as shown in Figure 1.11. To obtain decent yields in excess of, say, 80% for a 10-A Schottky device, micropipe densities must be in the order of 8 mp/cm2. For a 50-A Schottky one would need material with a micropipe density better than 2 mp/cm2. 100 100 4A 6A 4A 80 8A 10A 95 6A 15A 20A Yield (%) Yield (%) 90 8A 60 50A 100A 10A 85 15A 40 80 20A 20 50A 75 100A 0 70 0 20 40 60 80 100 0 5 10 Micropipe density Micropipe density Figure 1.11 Simulation of the yield of various sizes of Schottky diodes versus micropipe density for randomly distributed micropipes. The right-hand figure is a detail of the left-hand figure. Micropipes located on the active area or JTE region render a failed device, however, micropipes located in between the devices are considered harmless.
22 Silicon Carbide Overview Figure 1.11 is a simulation of randomly distributed micropipes, however, there is normally a tendency to cluster the micropipes, which would give somewhat better yields. Also, a significant amount of micropipes land in between the devices where the wafers are diced and these are considered harmless in the simulation. There is interesting research going on with respect to minimizing the micropipes by growing boules on the  plane . The plan is to let the micropipes and stacking faults propagate diagonally to prevent them from reaching the top surface of the boule. The researchers did indeed find micropipe-free areas and it will be interesting to follow future work on this. Similar research has been done on planes perpendicular to the  basal plane. Micropipe-free material has been grown, however, new defects appear as reported by the authors . 1.6.2 Stacking Faults The second defect that needs to be discussed does not have as grand a history as micropipes because it only recently became popular. This defect is the stacking fault, which creates degradation of bipolar devices. Reports by Lendenmann  and Bergman  reveal that a PiN diode operating under normal conditions begins to degrade. While the diode is operating, defects, which the authors interpret as stack- ing faults, evolve with an accompanying reduction in carrier lifetime. The defects thus act as recombination centers for the carriers. Furthermore, the stacking order has been identified as that of the 3C-SiC poly- type and, according to the study by Stahlbush, an explanation to the recombinative behavior of the stacking fault is that the 3C-SiC, having a lower bandgap than 4H- SiC, acts as a quantum well, thereby enhancing the recombination . It is a very serious materials issue that must be solved prior to the realization of commercial bipolar devices. Work is ongoing to reduce defects in SiC material. One of the more interesting concepts is the reduction of defects through epitaxial growth on porous SiC sub- strates . This approach has clearly demonstrated a reduction in intrinsic defects, as evidenced by photoluminescence measurements. It is too early to tell whether this technique can provide a path forward for the bipolar devices but it will clearly find its applicability in several areas where SiC will have a market.1.7 Commercial Outlook Silicon carbide has a clear place in society today, yet it has only one major commer- cial application today, which basically is materials or, more specifically, substrates for LED applications. This is perhaps not such a glamorous place to be in the com- mercial market but it does represent a significant starting point for SiC. The military has had SiC on its radar screen for many years for radar applica- tions, electronic warfare, more electric airplanes, more electric ships, more electric combat vehicles, and rail guns (which, we suppose, are also of the “more electric” variety). These applications require high-quality materials and large wafer sizes. Thanks to the military and its requirements for large wafers of high quality, the
1.7 Commercial Outlook 23 commercial SiC sector has started to wake up and aggressively pursue product development to meet these needs. 1.7.1 High-Frequency Applications Cree is currently offering MESFET devices geared toward the cellular base station market. It is estimated by Rutberg and Co. that the RF transistor market will be as large as $1.9 billion by 2006. Cell-phone base stations are clearly the biggest market for high-frequency devices. It will not be meaningful to replace all the transistors in a base station with SiC MESFETs or GaN high-electron mobility transistors (HEMTs), but a conservative estimate is that SiC will capture about 20% of this market, which would be approximately $400 million. However, due to the advan- tages of using SiC (or GaN), a higher average selling price (ASP) will be accepted by customers and it is therefore more accurate to estimate the SiC and GaN high- frequency market to be in excess of $1 billion. A recently published and interesting market study by Yole Développement esti- mates the high-frequency market for SiC MESFETs to be $400 million in 2007 . This also takes into account a dramatic annual price reduction of the components. The jury is still out whether it will be SiC MESFETs or GaN HEMTs that cap- ture the bulk of this large market. Silicon carbide MESFETs have overcome their ini- tial technological problems and have a clear potential to capture this market. However, GaN HEMTs show the highest power densities and highest frequency capabilities but are marred by an unfortunate instability caused by highly faulted materials. A GaN substrate would be a help in this respect but it would need to be semi- insulating. In addition, GaN has a poor thermal conductivity and is not very suit- able due to this negative material property. Aluminum nitride substrates may become the substrate of choice for GaN high-frequency applications. It has a rea- sonable thermal conductivity and is intrinsically semi-insulating but only time will tell. Unlike SiC, GaN is still not mature for the market. There is no doubt that the technological issues will be overcome but it will take some time. And finally, since money rules in the ruthless commercial world, will the manufacturing cost of GaN HEMTs be low enough to capture a lion’s share or just a niche portion of the market? 18.104.22.168 High-Power Applications By far the biggest application for SiC technology is the high-power electronics mar- ket. It may not be as glamorous as the high-frequency or the optoelectronic markets but it is big. The current size of the power-device market is $16 billion  and it is growing at a rate of almost 10% per year . The question on everyone’s mind is how big will the SiC share be? When determining where the power is used, it may come as a surprise that most power is used in a relatively narrow range between a couple of hundred volts to a couple of thousand volts and between an amp to several hundred amps, as can be seen in Figure 1.12. This range lies within the sweet spot for SiC unipolar devices.
24 Silicon Carbide Overview 10,000 HVDC and power 1,000 transmission Traction control Device Current (A) control Motor 100 60% Power supplies and factory automation 15% 10 Others Lamp ballast 25% 10 100 1,000 10,000 100,000 Device Blocking Voltage (V) Figure 1.12 The application for power devices relative to their blocking voltage and current ratings. Most power is used in a comparatively narrow range of voltage (200–2,000V) and between 1A to sev- eral hundred amps. This lies within the sweet spot for SiC unipolar devices. (After: .) Thus, if we begin substituting the old-fashioned Si devices with fresh new ultra-fast SiC unipolar devices, more than 75% of the power will go through an SiC device. This will be a major deal for the power industry on account of the superior per- formance of the SiC devices. If we assume that we improve the efficiency of the Si cir- cuits with another 5%, approximately $50 billion will be saved in power consumption annually in the United States as a result. On top of this are additional savings due to the fact that the air-conditioning needed to remove the heat that is no longer generated is dramatically reduced. Unfortunately, where the power is used is not where the bulk of power devices are sold. Most devices that are sold are for low-voltage (below 300V) and low- current applications in markets where SiC is not competitive. In the range between 300–600V, the picture is a little different, as can be seen in Figure 1.13. Approximately one-third of this market will be accessible for SiC (i.e., $1.32 billion of the Si share). Above 600V, it is estimated that SiC will capture 70% of the market (i.e., $1.68 billion of the Si share). As with high-frequency applications, the power-device market can support the higher ASP of SiC power devices. A factor of approximately 3–5 times higher ASP is expected. Thus, the $3 billion Si share would convert into an approximately $10 bil- lion SiC power-device share when the market is fully developed. A customer will be willing to pay a higher price for the SiC devices because there will be significantly larger savings on the passive components and on the cooling devices due to the higher switching frequency and increased efficiency. The market study by Yole estimates the SiC power-device market to be close to $600 million in 2007 and growing rapidly. This also covers bipolar devices, which are at higher voltages. Infineon, as well as Cree, has already launched its first power-device prod- ucts—Schottky diodes. The SiC Schottky diode market alone is estimated to be around $250 million by 2007. An interesting observation with respect to SiC